#------------------------------------------------------------------------------
#$Date: 2021-04-28 10:41:02 +0300 (Wed, 28 Apr 2021) $
#$Revision: 264624 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/21/1562192.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1562192
loop_
_publ_author_name
'Moetakef, Pouya'
'Larson, Amber M.'
'Hodges, Brenna C.'
'Zavalij, Peter'
'Gaskell, Karen J.'
'Piccoli, Philip M.'
'Rodriguez, Efrain E.'
_publ_section_title
;
 Synthesis and crystal chemistry of microporous titanates K (Ti,M)8O16
 where M=Sc--Ni
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              45
_journal_page_last               53
_journal_paper_doi               10.1016/j.jssc.2014.08.012
_journal_volume                  220
_journal_year                    2014
_chemical_compound_source        Synthesized
_chemical_formula_sum            'Fe1.52 K1.53 O16 Ti6.48'
_chemical_formula_weight         710.91
_space_group_crystal_system      tetragonal
_space_group_IT_number           87
_space_group_name_Hall           '-I 4'
_space_group_name_H-M_alt        'I 4/m'
_space_group_ssg_IT_number       87
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      87
_symmetry_space_group_name_H-M   'I 4/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   10.153214(97)
_cell_length_b                   10.153214(97)
_cell_length_c                   2.967320(33)
_cell_measurement_temperature    300
_cell_volume                     305.894(5)
_computing_cell_refinement       'Bruker AXS TOPAS 4.2'
_computing_structure_refinement  'Bruker AXS TOPAS 4.2'
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type  'Bruker D8'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.5418
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       3
_diffrn_reflns_limit_l_min       0
_diffrn_source                   'Sealed X-ray tube'
_exptl_absorpt_coefficient_mu    53.887
_exptl_crystal_colour            Red
_exptl_crystal_density_diffrn    3.859
_pd_char_colour                  Red
_pd_meas_2theta_range_inc        0.0092
_pd_meas_2theta_range_max        140
_pd_meas_2theta_range_min        7
_pd_meas_number_of_points        14449
_pd_proc_2theta_range_inc        0.0092
_pd_proc_2theta_range_max        140
_pd_proc_2theta_range_min        7
_pd_proc_ls_background_function
;   One on X                                 125680(440)
   Chebychev polynomial, Coefficient  0      -2334(14)
                                      1      3585(17)
                                      2      -1874(11)
                                      3      988.4(63)
                                      4      -477.2(38)
                                      5      194.6(20)
                                      6      -69.5(13)

;
_pd_proc_ls_pref_orient_corr     '(Dir 1 : 0 0 1)     1.3247(19)'
_pd_proc_ls_prof_R_factor        3.52
_pd_proc_ls_prof_wR_expected     2.80
_pd_proc_ls_prof_wR_factor       4.56
_refine_ls_goodness_of_fit_all   1.63
_refine_ls_number_constraints    6
_refine_ls_number_parameters     25
_refine_ls_R_I_factor            2.011
_cod_data_source_file            JSSC-2014-220-45-1.cif
_cod_data_source_block           KTFO
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_geom_angle_publ_flag' value 'N' was changed to 'n' in
accordance with the built-in table derived from the CIF Core
dictionary named 'cif_core.dic' version 2.4.5 last updated on
2014-11-21 (20 times).

data item '_geom_bond_publ_flag' value 'N' was changed to 'n' in
accordance with the built-in table derived from the CIF Core
dictionary named 'cif_core.dic' version 2.4.5 last updated on
2014-11-21 (12 times).

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_cell_volume        305.8944(68)
_cod_original_sg_symbol_H-M      I4/m
_cod_database_code               1562192
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_symmetry_multiplicity
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Ti1 Ti 8 0.646858(99) 0.16807(12) 0 0.81 0.459(22)
Fe1 Fe 8 0.646858(99) 0.16807(12) 0 0.19 0.459(22)
O1 O 8 0.66049(31) 0.03784(35) 0.5 1 0.459(22)
O2 O 8 0.65527(33) 0.29321(32) 0.5 1 0.459(22)
K1 K 4 0.5 0.5 0.2300(60) 0.2260(71) 0.459(22)
K2 K 2 0.5 0.5 0 0.313(14) 0.459(22)
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_publ_flag
Ti1 O1 O2 48.31(7) n
Ti1 O1 K1 40.6(2) n
Ti1 O1 K2 33.30(6) n
Ti1 O2 O1 49.55(7) n
Ti1 O2 K1 104.5(3) n
Ti1 O2 K2 93.22(6) n
Ti1 K1 O1 20.21(7) n
Ti1 K1 O2 30.34(9) n
Ti1 K1 K2 79.5(3) n
Ti1 K2 O1 17.27(1) n
Ti1 K2 O2 31.99(4) n
Ti1 K2 K1 90.0 n
K1 O1 O2 20.11(11) n
K1 O1 K2 7.5(2) n
K1 O2 O1 140.93(18) n
K1 O2 K2 12.5(4) n
K1 K2 O1 73.37(1) n
K1 K2 O2 60.53(3) n
K2 O1 O2 24.31(5) n
K2 O2 O1 134.90(9) n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_publ_flag
Ti1 O1 1.993(2) n
Ti1 O2 1.955(2) n
O1 Ti1 1.993(2) n
O1 O2 2.594(4) n
O2 Ti1 1.955(2) n
O2 O1 2.594(4) n
O2 K1 2.745(6) n
O2 K2 3.016(3) n
K1 K2 0.683(18) n
K1 O2 2.745(6) n
K2 K1 0.683(18) n
K2 O2 3.016(3) n
